# Synthesis and optimization of biobased carbon adsorbent monoliths from chitosan-polybenzoxazine for efficient CO2 capture

José Mosquera, Liana Delevingne, Frédéric Delbecq, Elias Daouk, Audrey

Drelich, Khashayar Saleh, Rémi Gautier, Mikel Leturia

► To cite this version:

José Mosquera, Liana Delevingne, Frédéric Delbecq, Elias Daouk, Audrey Drelich, et al. Synthesis and optimization of biobased carbon adsorbent monoliths from chitosan-polybenzoxazine for efficient CO2 capture. RSC Advances, 2025, 15 (9), pp.6783-6793. 10.1039/D5RA00110B. hal-04976953

HAL Id: hal-04976953

https://hal.science/hal-04976953v1

Submitted on 7 Nov 2025

HAL is a multi-disciplinary open access
archive for the deposit and dissemination of sci-
entific research documents, whether they are pub-
lished or not. The documents may come from
teaching and research institutions in France or
abroad, or from public or private research centers.

L'archive ouverte pluridisciplinaire HAL, est
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d'enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.

<figure><img src="image_1.png" /></figure>

Distributed under a Creative Commons Attribution 4.0 International License
<figure><img src="image_2.png" /></figure>

Check for updates

Cite this: RSC Adv., 2025, 15, 6783

# Synthesis and optimization of biobased carbon adsorbent monoliths from chitosan-polybenzoxazine for efficient CO₂ capture

José E. Mosquera,ª Liana Delevingne,ª Frédéric Delbecq,ª Elias Daouk,ª Audrey Drelich,ª Khashayar Saleh,ª Rémi Gautierᵇ and Mikel Leturia ID*ª

The present study introduces a novel method for the preparation of a CO₂ carbon adsorbent derived from biobased precursors. Porous carbon adsorbents were synthesized through the carbonization and thermal activation of biobased chitosan-polybenzoxazine. First, the study explored the influence of varying amounts of the key polymer precursors, lysine (0.05–0.1 g) and chitosan (0.6–0.12 g), on the surface and adsorption characteristics of the obtained carbons. This aimed to identify the most favourable amounts of these precursors that resulted in the highest CO₂ adsorption performance. In the subsequent stage, the study investigated the impact of different activation times (1–7 h) to enhance the surface characteristics and CO₂ adsorption capacity of the activated carbon. Both carbonization and activation processes were conducted in a tubular furnace at 900 °C under N₂ and CO₂ atmospheres, respectively. After carbonization, the resulting carbon monoliths exhibited a char yield of approximately 49 wt%, with a BET surface area of up to 541 m² g⁻¹ and a CO₂ uptake of 4.0 mmol g⁻¹ at 0 °C and 1 bar. After activation, the obtained samples displayed a surface area in the range of 650–1000 m² g⁻¹, with CO₂ adsorption capacities at 1 bar ranging from 4.5 to 5.6 mmol g⁻¹ at 0 °C and 3.2 to 4 mmol g⁻¹ at 25 °C. The activated carbons also demonstrated excellent selectivities for CO₂/N₂ and CO₂/CH₄ mixtures, along with a stable CO₂ adsorption–desorption performance after 10 cycles.

Received 6th January 2025
Accepted 25th February 2025

DOI: 10.1039/d5ra00110b

rsc.li/rsc-advances

## 1. Introduction

Over the past few decades, global warming has emerged as a critical concern due to increasing levels of greenhouse gases in the atmosphere, primarily caused by the use of fossil carbon resources in energy, industry and transportation.¹ In particular, carbon dioxide (CO₂) is widely regarded as the foremost contributor to the global rise in mean temperatures.² As a result, numerous researchers have focused their efforts on developing efficient methods for CO₂ capture and storage. These efforts aim not only to reduce CO₂ emissions but also to create strategies for enhancing the selective separation of CO₂ from complex gas mixtures. Recently, various CO₂ capture technologies have been under investigation, including chemical absorption, adsorption and membrane separation.³⁻⁶

Among these technologies, CO₂ adsorption by solid porous materials has received significant attention, owing to its numerous advantages, including chemical stability, ease of recovery and high adsorption capacity, even under humid conditions.⁷⁻⁹ Recent studies have further demonstrated that

carbon adsorbents exhibit excellent CO₂ adsorption capacity and selectivity.¹⁰⁻¹² Porous carbon materials can be produced through the pyrolysis of various polymeric precursors including polymers of natural origin, as well as synthetic polymers such as polyamide, polyacrylonitrile, phenolic resin and polymer blends.⁸,¹³ Despite the development of numerous carbonized materials, there is a strong trend toward creating new adsorbent materials from bioresource-derived precursors with superior adsorption capacity. This trend continues to open up opportunities for further advancements in this type of material.

Renewable resources and bio-based raw materials have been successfully utilized as precursors for producing carbon adsorbents, including wood,¹⁴ chitosan,¹⁵ polysaccharides¹⁶ and lignin,¹⁷ among others, showcasing promising results for CO₂ capture. Additionally, N-doped carbon frameworks produced from several biomass-derived precursors have shown enhanced CO₂ adsorption performance under ambient conditions.¹⁸⁻²⁰

Polybenzoxazines (PBZ) are a class of phenolic thermosetting resins typically synthesized through a cationic ring-opening polymerization of benzoxazine monomers, forming a cross-linked network of tertiary amine bridges. They can be synthesized from cost-effective raw materials, including primary amines, phenol sources and formaldehyde.⁸,¹¹,²⁰⁻²⁴ These materials are distinguished from traditional polymers by their exceptional features, such as good chemical and electrical

<figure><img src="image_3.png" /></figure>

<footnote>ªUniversité de Technologie de Compiègne, ESCOM, TIMR, Compiègne, France. E-mail: mikel.leturia@utc.fr; Tel: +33 6 28 23 87 85</footnote>

<footnote>ᵇIMT Nord Europe, Institut Mines-Télécom, CERI Energie et Environnement, F-59508 Douai, France</footnote>
<table><caption>**Table 1** Comparison of the CO₂ adsorption capacity of different PBZ-based porous carbon materials from the literature</caption><thead><tr><th>Author</th><th>S<sub>BET</sub><br>[m<sup>2</sup> g<sup>-1</sup>]</th><th>CO<sub>2</sub> uptake at 0 °C and 1 bar<br>[mmol g<sup>-1</sup>]</th></tr></thead><tbody><tr><td>Present work</td><td>998</td><td>5.60</td></tr><tr><td>Konnola<sup>23</sup></td><td>910</td><td>4.25</td></tr><tr><td>Jin<sup>30</sup></td><td>1720</td><td>6.96</td></tr><tr><td>Zhang<sup>33</sup></td><td>815</td><td>7.00</td></tr><tr><td>Guo<sup>34</sup></td><td>1292</td><td>7.04</td></tr><tr><td>Hao<sup>20</sup></td><td>1392</td><td>4.90</td></tr><tr><td>Hong<sup>22</sup></td><td>2423</td><td>8.44</td></tr><tr><td>Samy<sup>18</sup></td><td>560</td><td>6.81</td></tr><tr><td>Xia<sup>35</sup></td><td>3360</td><td>6.92</td></tr></tbody></table>

resistance, high thermal stability, good mechanical strength, high char yields, low water adsorption, minimal shrinkage during curing and flame retardancy.18,25–29 These unique qualities extend the utility of PBZ across various applications, from serving as adsorbents for CO₂,21,30 water treatment31 and also electronics and aerospace industries.16,32 In recent times, there has been a growing interest in polybenzoxazines derived from renewable bioresource materials.25 Notably, benzoxazine molecules have been synthesized using green solvents, such as water and aqueous solutions.26 In this work, we will explore the development of chitosan-based polybenzoxazine-derived carbon materials for CO₂ capture. For comparison, Table 1 summarizes the CO₂ adsorption capacity of various polybenzoxazine-derived carbon materials reported in the literature.

Chitosan (2-amino-2-deoxy-D-glucopyranose) is a natural polymer, primarily derived from the exoskeletons of crab and shrimp shells.28 It is soluble in acidic solvents having a pH value lower pH 6.0.36 This biopolymer has attracted enormous interest due to its advantageous characteristics, which include reactive functionality, a high concentration of amine groups, low production costs, widespread availability, low toxicity and environmental friendliness.28,37 Consequently, chitosan finds applications in various domains, ranging from drug delivery systems,38 separation membrane39 to active food packaging.40 Several carbon adsorbents derived from chitosan-based precursors for CO₂ capture have been reported. For instance, Witoon et al.41 synthesized a meso–macroporous polyethyleneimine-loaded silica monolith using chitosan as a biotemplate. The resulting carbon product exhibited a BET surface area of 246 m² g⁻¹ and a CO₂ adsorption capacity of 3.8 mmol g⁻¹ at 80 °C. Alhwaige et al.42 fabricated chitosan-graphene oxide hybrid aerogels through a freeze-drying method. The resulting carbon possessed a BET surface area of 415 m² g⁻¹ and a CO₂ adsorption capacity of 4.15 mmol g⁻¹ at 25 °C and 1 bar pressure. In a subsequent study, the authors prepared a carbon aerogel from clay-reinforced biobased chitosan-polybenzoxazine using the same method, yielding a carbon material with high surface areas (up to 710 m² g⁻¹) and excellent adsorption performance of 5.72 mmol g⁻¹ at 25 °C and 1 bar.19 Kamran et al.43 developed chitosan-based porous

carbons through hydrothermal carbonization and chemical activation with KOH and NaOH. The products displayed a superior surface area of 4168 m² g⁻¹ and a maximum CO₂ uptake of 8.36 mmol g⁻¹ at 0 °C and 1 bar. Ghimbeu and Luchnikov15 produced nitrogen-doped carbonized beads from chitosan acetate, cross-linkers and Pluronic F127 co-solution drops. After freeze-drying and carbonization, the resulting carbon achieved a surface area of 433 m² g⁻¹ and a CO₂ uptake of 2.85 mmol g⁻¹ at 0 °C at 1 bar.

Within the preceding scope, the present study reports a simple, scalable and eco-friendly approach for preparing carbon adsorbent monoliths for CO₂ adsorption. The formation of carbon monoliths is achieved through the utilization of biobased precursors, wherein chitosan serves as both a biotemplating and nitrogen source, lysine functions as a polymerization agent, and water serves as the exclusive solvent. Subsequently, the resulting polymer monolith undergoes drying at 75 °C, followed by carbonization and thermal activation. Therefore, the aim of this work is to fabricate a porous carbon monolith derived from chitosan-polybenzoxazine, and enhance its properties by thermal activation, including surface characteristics and adsorption capacity. The production yields, CO₂/N₂ and CO₂/CH₄ selectivities, as well as adsorption/desorption cyclability are also evaluated. It is noteworthy that this study highlights a method with the following key advantages: it mainly uses sustainable biobased precursors, still offering simplicity and scalability, and includes optimized formulation and fabrication processes, making it well suited for industrial applications.

## 2. Materials and methods

### 2.1. Materials

Chitosan (≥75% deacetylated from shrimp), resorcinol (99.0%) and formalin (37 wt% in water), were purchased from Sigma-Aldrich Corp. Lysine (98%) was purchased from Acros Organics, and APG (alkyl polyglycoside C₈–C₁₀, trade name Plantacare® 2000 UP) from BASF. All chemicals were used as received.

### 2.2. Preparation of chitosan-PBZ carbon monolith

The chitosan-PBZ monolith was synthesized via a sol–gel process, as shown in Fig. 1. In a typical synthesis process, 0.2 g of APG was dissolved in 13 mL of deionized water, in a 50 mL flask with magnetic stirring under ambient conditions (step 1). Afterward, resorcinol (27.3 mmol, 3 g), lysine (0.1 g) and chitosan (0.9 g) were added to this solution. The mixture was vigorously stirred until complete dissolution of resorcinol and lysine, leaving a uniform suspension of chitosan (step 2). The resulting suspension was poured into a 25 mL plastic syringe and subsequently, formaldehyde (54.5 mmol, 1.63 g, corresponding to 4 mL of formalin at 37 wt% in water) was quickly added to the solution (step 3). Then, the syringe containing the suspension was vigorously agitated and placed vertically in an oven, preheated to 75 °C for 2 hours (step 4). After that, the remaining liquid and the syringe plunger were removed, and

<figure><img src="image_4.png" /></figure>
<figure><img src="image_5.png" /></figure>

<figure><img src="image_6.png" /><figcaption>Fig. 1 Schematic of the experimental procedure for activated carbon preparation.</figcaption></figure>

the syringe barrel was returned to the oven at the same temperature, for an additional 48 hours to achieve complete drying (step 5).

The as-prepared polymer monolith was extracted from the syringe and pyrolyzed for 2 hours in a tubular furnace at 900 °C (with a heating rate of 5 °C min⁻¹), under nitrogen atmosphere (with a gas flow rate of 200 mL min⁻¹) (step 6). In this work, the selection of the pyrolysis temperature (900 °C), heating rate (5 °C min⁻¹) and hold time (2 hours) was based on a comprehensive review of existing literature, preliminary experiments, and insights derived from prior research.⁴⁴

As a first study, three polymer monoliths were prepared, each with different amounts of chitosan and lysine (corresponding to low, medium and high concentrations, as detailed in Table 2), while the mass of the remaining precursors stayed constant. These polymer monoliths were denoted as PCHL-x (polybenzoxazine-chitosan-lysine), where “x” indicates the concentration level of chitosan and lysine in the resulting material (x = 1 for low concentration, x = 2 for medium concentration and x = 3 for high concentration). Subsequently, the three polymer monoliths were pyrolyzed and the CO₂ adsorption capacity of the obtained porous carbons was characterized (characterization techniques are detailed in section 2.3).

As a second study, the pyrolyzed sample displaying the highest CO₂ adsorption capacity was chosen for further investigation regarding the subsequent thermal activation step. In order to optimize the surface characteristics and adsorption capacity, different activation times (1, 3, 5 and 7 hours) were applied to the pyrolyzed monolith previously selected. In all these experiments, the carbon monolith was heated from room

temperature to 900 °C, with a ramp rate of 20 °C min⁻¹ under nitrogen atmosphere.

The flowing gas was subsequently switched from nitrogen to a gas mixture of CO₂/N₂ (20/80 molar%), maintained for the selected activation time, and then switched back to nitrogen, all at the same flow rate (200 mL min⁻¹). The resulting activated carbons were designated as ACP-x-y (activated carbon polybenzoxazine), where “x” indicates the concentration level of chitosan and lysine in the polymer monolith, and “y” refers to the activation time (in hours).

## 2.3. Characterization techniques

Fourier Transform Infrared (FTIR) spectroscopy was used to identify the functional groups of the PBZ materials and the porous carbons, using a Thermo Scientific Nicolet iS5 with iD1 transmission FTIR spectrometer (Thermo 190 Scientific®, USA) at room temperature in the range of 400–4000 cm⁻¹ at a resolution of 4 cm⁻¹, with a KBr pellet. Elemental analysis was carried out on a Thermo Scientific Flash 2000 CHNS/O Analyzer (Thermo Fisher Scientific, USA). The surface topography of porous carbon materials was observed by Scanning Electron Microscopy (SEM), with a FEI Quanta 3D FIB FEG instrument operated at 20 kV. A 3Flex sorption analyser (Micromeritics, Norcross, GA, USA) was used to assess the surface characteristics and gas adsorption properties, by measuring the isotherms for CO₂, N₂ and CH₄. N₂ adsorption/desorption isotherms were conducted at -196 °C using nitrogen (99.998% purity), after degassing the porous carbons at 220 °C for 20 h. The specific surface area (S<sub>BET</sub>) was calculated from the N₂ adsorption isotherm by using the Brunauer–Emmett–Teller (BET) method, while the pore size distribution was estimated with the Horvath–Kawazoe (HK) method. The total pore volume (V<sub>total</sub>) was calculated from the amount of N₂ adsorbed at a relative pressure of 0.99. Micropore volume (V<sub>mic</sub>) and micropore surface area (S<sub>mic</sub>) were calculated using the t-plot method. The adsorption isotherms of CO₂, N₂ and CH₄ were conducted at three different temperatures (0, 25 and 50 °C) in the pressure range of 0 to 1 bar. Prior to each adsorption test, the samples were degassed at 220 °C for at least 6 hours.

<table><caption>**Table 2** Concentration levels of chitosan and lysine in the polymer monoliths</caption><thead><tr><td>Sample name</td><td>Concentration level</td><td>Chitosan [g]</td><td>Lysine [g]</td></tr></thead><tbody><tr><td>PCHL-1</td><td>Low</td><td>0.6</td><td>0.05</td></tr><tr><td>PCHL-2</td><td>Medium</td><td>0.9</td><td>0.1</td></tr><tr><td>PCHL-3</td><td>High</td><td>1.2</td><td>0.15</td></tr></tbody></table>
<figure><img src="image_7.png" /></figure>

The char yield refers to the amount of carbon obtained after the carbonization process, expressed as a percentage of the initial mass of the precursor material. It was calculated based on the following equation:

$$ \text{Char yield (\%)} = \frac{w_c}{w_0} \times 100 \qquad (1) $$

where $w_0$ (g) and $w_c$ (g) are the initial mass of the precursor and mass of the carbon material after pyrolysis, respectively.

The burn-off reflects the activation progress and is calculated as the percentage of mass lost during the activation of the carbonized material:

$$ \text{Bo}(\%) = \text{Burn-off}(\%) = \frac{w_c - w_a}{w_c} \times 100 \qquad (2) $$

where $w_a$ (g) is the final mass of activated material (i.e., mass after activation).

The activation process leads to a higher surface area but also results in a mass loss of the activated product (burn-off). Thus, determining the optimal balance between CO₂ adsorption capacity and available mass of activated carbon is crucial. To address this, we introduce the concept of “available CO₂ adsorption capacity”, expressed in mmol of CO₂ per gram of pyrolyzed material. This requires converting the CO₂ adsorbed per unit mass of activated material (denoted as $A_c$) into CO₂ adsorbed per unit mass of pyrolyzed material. Consequently, the available CO₂ adsorption capacity is calculated as:

$$ \text{Available CO}_2 \text{ capacity} = A_c \left( 1 - \frac{\text{Bo}(\%)}{100} \right) \qquad (3) $$

where $A_c$ (mmol of CO₂ g⁻¹ of activated material) is the CO₂ adsorption capacity of the activated material and Bo is the burn-off (%) after activation.

The CO₂/N₂ and CO₂/CH₄ selectivities of the carbon adsorbed were calculated using the Ideal Adsorbed Solution Theory (IAST),⁵,²² given by:

$$ S_{\text{ads}} = \frac{q_1/q_2}{P_1/P_2} \qquad (4) $$

where $q_i$ is the amount of gas i adsorbed (mmol g⁻¹) and $P_i$ is the partial pressure (bar) of gas i in the mixture.

# 3. Results and discussion

## 3.1. Structural properties of the polymer and porous carbon monoliths

Porous carbon monoliths were successfully prepared from chitosan-PBZ polymers. In Fig. 2a, a representative example of chitosan-PBZ polymer monolith and its carbonized counterpart are presented. Notably, the carbonization process yields a crack-free carbon monolith that retains a uniform shape, similar to the original polymer structure. The resulting carbon monolith typically exhibits dimensions of 31 mm in length and 15 mm in diameter, which corresponds to an overall volume shrinkage of 60%. SEM images (Fig. 2b and c) further illustrate that both the polymer and carbon materials consist of interconnected microspheres and possibly amorphous solid, forming a micro-porous framework. The FTIR spectra of both the precursor

<figure><img src="image_8.png" /><figcaption>Fig. 2 (a) Representative photographs of polymer and carbon monoliths; (b) and (c) SEM images of resin and carbonized materials, respectively; (d) FTIR spectra of resin and carbonized materials.</figcaption></figure>

polymer and the porous carbon are presented in Fig. 2d. The FTIR spectrum of chitosan-PBZ resin exhibits characteristic absorption peaks in the range of 3400–3200 cm⁻¹ attributed to the O–H bonds and/or N–H stretching vibrations of chitosan amide groups.³⁹ Additionally, bands at 2922 cm⁻¹ and 2847 cm⁻¹ correspond to C–H bending. The absorption peaks in the range of 1600 cm⁻¹ and 1485 cm⁻¹ can be attributed to C=C and C–C within the aromatic rings of the benzoxazine structure.³⁰,⁴⁵ Furthermore, the bands observed at 1240 and 1160 cm⁻¹ were assigned to asymmetric and symmetric stretching of the oxazine structure C–O–C.²⁷ Moreover, a band around 1110 cm⁻¹ suggests the presence of the C–N stretching vibrations,⁴⁶ while the weak absorption bands occurring at 926, 874 and 764 cm⁻¹ are indicative of C–H groups.

## 3.2. Effect of chitosan and lysine concentrations

As noted earlier, three monoliths with varying amounts of lysine and chitosan were synthesized and carbonized (while the mass of the remaining precursors stayed constant). The CO₂ adsorption isotherms, measured at 0 °C, are illustrated in Fig. 3. The highest CO₂ uptake capacity at 0 °C was achieved with the PCHL-2 sample. To understand this behaviour, Table 3 presents the key characteristics of the three monoliths. The data reveals an almost constant char yield for all the samples of approximately 49 wt%. In addition, elemental analysis demonstrated an increase in nitrogen content with the addition of chitosan and lysine, ranging from 1.7 to 2.3 wt%. This observation aligns with expectations, considering that both precursors can be considered as nitrogen sources. Furthermore, the results (Table 3 and Fig. 3) reveal that the highest BET surface area
<figure><img src="image_9.png" /></figure>

<figure><img src="image_10.png" /><figcaption>Fig. 3 CO₂ adsorption isotherms at 0 °C of chitosan-based porous carbon monoliths.</figcaption></figure>

(541 m² g⁻¹) and CO₂ uptake capacity at 0 °C and 1 bar (4.05 mmol g⁻¹) were achieved with the PCHL-2 sample. These results suggest that the cross-linking of chitosan and lysine at an intermediate concentration level results in an optimized carbon framework structure, with increased surface area and active sites for CO₂ adsorption.

According to the work of Sun *et al.*,⁴⁷ a structured network made of chitosan and other elements, such as amino acids, could generate nitrogen-enriched substructures, including pyridinic or graphitic moieties, after pyrolysis. These substructures are reported to be important for the stabilization of the CO₂ uptake. Consequently, the PCHL-2 formula was selected as the preferred material for the subsequent thermal activation experiments.

### 3.3. Effect of activation progress

The carbon material obtained after pyrolysis of the chitosan-PBZ polymer was subjected to activation with CO₂ at 900 °C, in order to enhance its surface characteristics and CO₂ adsorption capacity. The evolution of the textural properties (specific surface area, micropore surface area, total and micropore volumes) with activation progress (i.e., burn-off) is summarized in Table 4, together with the CO₂ adsorption capacity and elemental analysis.

First, it is evident that the burn-off increases with activation time, ranging from 5% to 23% within the studied time range (1 to 7 hours). This increase is expected due to the extended contact time between CO₂ and the carbon material during the activation treatment. However, the resulting activated carbon monoliths did not show any significant modifications in their physical structure during the activation process, as the shrinkage did not exceed 5% under all studied conditions. In the same way, there is no clear trend observed in the elemental composition, particularly in terms of nitrogen content. The samples still contain approximately 2 wt% of nitrogen after activation. These nitrogen content values are of interest due to the potential role that N heteroatoms can play in CO₂ capture.⁸,⁴⁸

The nitrogen adsorption/desorption isotherms and the corresponding pore-size distributions of the obtained carbon materials are displayed in Fig. 4a and b, respectively. As shown in Fig. 4a, the porous carbon materials exhibit typical type-I isotherms, with a rapid increase of N₂ sorption at low relative pressures (<0.05), indicating the predominance of micropores for all of these samples.

From Table 4, a progressive increase of the main surface characteristics (specific surface area, micropore surface area,

<table><caption>Table 3 Adsorption characteristics of chitosan-based porous carbon monoliths</caption><thead><tr><th rowspan="2">Sample</th><th rowspan="2">Chitosan and lysine concentration level</th><th rowspan="2">Char yield [%]</th><th rowspan="2">S<sub>BET</sub> [m<sup>2</sup> g<sup>-1</sup>]</th><th rowspan="2">CO<sub>2</sub> uptake at 0 °C and 1 bar [mmol g<sup>-1</sup>]</th><th colspan="3">Elemental analysis (wt%)</th></tr><tr><th>N</th><th>C</th><th>H</th></tr></thead><tbody><tr><td>PCHL-1</td><td>Low</td><td>51%</td><td>489</td><td>3.36</td><td>1.73</td><td>93.41</td><td>0.40</td></tr><tr><td>PCHL-2</td><td>Medium</td><td>49%</td><td>541</td><td>4.05</td><td>2.07</td><td>91.47</td><td>0.37</td></tr><tr><td>PCHL-3</td><td>High</td><td>47%</td><td>506</td><td>3.66</td><td>2.30</td><td>93.70</td><td>0.41</td></tr></tbody></table>

<table><caption>Table 4 Textural and adsorption properties of porous carbons at different stages of activation</caption><thead><tr><th rowspan="2">Sample</th><th rowspan="2">Burn-off [%]</th><th rowspan="2">S<sub>BET</sub><sup>a</sup> [m<sup>2</sup> g<sup>-1</sup>]</th><th rowspan="2">S<sub>mic</sub><sup>b</sup> [m<sup>2</sup> g<sup>-1</sup>]</th><th rowspan="2">V<sub>total</sub><sup>c</sup> [cm<sup>3</sup> g<sup>-1</sup>]</th><th rowspan="2">V<sub>mic</sub><sup>d</sup> [cm<sup>3</sup> g<sup>-1</sup>]</th><th colspan="2">CO<sub>2</sub> uptake [mmol g<sup>-1</sup>]</th><th colspan="4">Elemental analysis [wt%]</th></tr><tr><th>0 °C</th><th>25 °C</th><th>N</th><th>C</th><th>H</th><th>O</th></tr></thead><tbody><tr><td>PCHL-2</td><td>0</td><td>541</td><td>501</td><td>0.28</td><td>0.25</td><td>4.05</td><td>3.25</td><td>2.07</td><td>91.47</td><td>0.37</td><td>1.53</td></tr><tr><td>ACP-2-1</td><td>5</td><td>660</td><td>622</td><td>0.33</td><td>0.32</td><td>4.52</td><td></td><td>2.16</td><td>91.74</td><td>0.53</td><td>1.22</td></tr><tr><td>ACP-2-3</td><td>12</td><td>930</td><td>845</td><td>0.46</td><td>0.42</td><td>5.22</td><td>3.99</td><td>1.98</td><td>92.60</td><td>0.49</td><td>1.11</td></tr><tr><td>ACP-2-5</td><td>17</td><td>995</td><td>888</td><td>0.49</td><td>0.45</td><td>5.44</td><td></td><td>1.87</td><td>92.48</td><td>0.42</td><td>1.02</td></tr><tr><td>ACP-2-7</td><td>23</td><td>998</td><td>902</td><td>0.50</td><td>0.46</td><td>5.60</td><td>3.95</td><td>1.84</td><td>92.32</td><td>0.42</td><td>1.29</td></tr></tbody></table>

<footnote>a BET specific surface area obtained from the adsorption data in the P/P₀ range from 0.05 to 0.2. b Microporous specific surface area obtained from t-plot method. c Total pore volume at a relative pressure of 0.99. d Micropore volume. The results are shown as mean values (n = 2 replicates).</footnote>
<figure><img src="image_11.png" /><figcaption>Fig. 4 (a) N₂ sorption isotherms for different activation times. (b) Pore size distributions (PSDs) calculated from the Horvath–Kawazoe method.</figcaption></figure>

total and micropore volumes) can be observed with the activa-
tion progress. For instance, S<sub>BET</sub> increased from 541 to 998 m²
g⁻¹, while V<sub>total</sub> increased from 0.28 to 0.50 cm³ g⁻¹. This trend
is consistent with findings in prior studies on CO₂ activation of
carbons.<sup>49–51</sup> The enhancement of these textural properties can
be attributed to the prolonged contact time between CO₂ and
the char, leading to increased burn-off and greater pore devel-
opment.<sup>52</sup> Also, it should be noted that the increase of the main
surface characteristics becomes slower in the later stages of
activation. The Horvath–Kawazoe micropore size distributions
of the obtained porous carbons are presented in Fig. 4b. The
majority of the micropores are concentrated in the 0.6–1.2 nm
range, with the cumulative pore volume increasing as activation
progresses. It can be concluded that thermal activation signif-
icantly improves the surface properties of the carbon material.
Notably, through this process, the activated carbon achieves up
to twice the specific surface area S<sub>BET</sub> and pore volume V<sub>total</sub>,
compared to the non-activated carbon.

Finally, the CO₂ adsorption capacity of the porous carbon
materials was investigated at 0 °C under atmospheric pressure

(1 bar). Table 4 provides a summary of the CO₂ uptakes and
Fig. 5 shows the CO₂ adsorption isotherms at 0 °C. From both
Table 4 and Fig. 5, it can be noticed that the CO₂ adsorption
capacity progressively increases with the activation progress.

The highest CO₂ adsorption capacity of 5.6 mmol g⁻¹ is achieved after 7 h of activation, corresponding to a burn-off of 23%. Notably, this represents an increase in adsorption capacity of up to 38% compared to non-activated carbon. This enhancement is consistent with the earlier trends observed for the BET surface area and pore volume. Furthermore, as the activation progresses, there is an enlargement of the micropore range, especially in the fraction of micropores smaller than 0.8 nm (Fig. 4b). This factor is likely to contribute to the improvement of CO₂ uptake, as the CO₂ adsorption capacity at 1 bar is highly dependent on the micropores in this size range.<sup>5,34,48,50</sup> It is also noteworthy that the resulting carbon materials exhibit a very high CO₂ uptake under ambient conditions, ranging from 3.25 to 4 mmol g⁻¹ at 25 °C and 1 bar.

3.4. Production yields of the carbon adsorbents

Fig. 6 shows the evolution of the BET surface area, CO₂ uptake (at 0 °C and 1 bar) and available CO₂ adsorption capacity of the activated carbons with burn-off. As explained in the previous section, the activation process leads to an enhancement of textural properties and CO₂ adsorption capacity (Fig. 6a and b). However, a higher activation progress also leads to a higher mass loss (burn-off), i.e., a lower quantity of the final adsorbent material. Therefore, in the context of industrial applications, it becomes imperative to identify the best compromise between CO₂ adsorption capacity and available mass of activated carbon. To this purpose, the available CO₂ adsorption capacity was calculated for all activated carbons, using eqn (3). Fig. 6c displays the CO₂ adsorption capacity per unit mass of pyrolyzed carbon as a function of the activation burn-off.

The obtained results show that the carbon adsorbent ACP-2-3, obtained after 3 hours of activation (corresponding to a burn-off of 12%), exhibits the best balance between adsorption capacity and mass loss. Accordingly, a recommended route for producing an optimal carbon adsorbent involves carbonizing at

<figure><img src="image_12.png" /><figcaption>Fig. 5 CO₂ adsorption isotherms at 0 °C for different activation times.</figcaption></figure>
<figure><img src="image_13.png" /></figure>

<figure><img src="image_14.png" /><figcaption>Fig. 6 Evolution of the (a) BET surface area, (b) CO₂ uptake (at 0 °C and 1 bar), and (c) available CO₂ adsorption capacity of the activated carbons with burn-off.</figcaption></figure>

900 °C the chitosan-PBZ monolith with an intermediate concentration of chitosan and lysine, followed by a 3 hour thermal activation process.

### 3.5. CO₂/N₂ and CO₂/CH₄ selectivities

A crucial aspect in the development of a CO₂ adsorbent is its ability to separate CO₂ from other gases, particularly N₂ (for CO₂ capture from flue gas streams) and CH₄ (for natural gas sweetening). Therefore, an effective adsorbent material with high adsorption performance should also exhibit a high CO₂ selectivity over N₂ and/or CH₄. As a consequence, the CO₂/N₂ and CO₂/CH₄ selectivities of the non-activated porous carbon (PCHL-2) and the chosen activated porous carbon (ACP-2-3) were investigated. To this end, the N₂ and CH₄ adsorption isotherms were characterized at three temperatures (0, 25 and 50 °C) for pressures ranging from 0 to 1 bar. The obtained results are presented in Fig. 7 and summarized in Table 5.

The N₂ (Fig. 7a and b) and CH₄ (Fig. 7c and d) adsorption capacities of PCHL-2 and ACP-2-3 measured at 1 bar pressure and 0 °C, 25 °C and 50 °C, range from 0.27 to 0.82 and 0.6 to 2.1 mmol g⁻¹, respectively. On the other hand, the CO₂ adsorption capacity for the same materials under the same conditions ranges from 1.9 to 5.2 mmol g⁻¹. This observation indicates significantly lower N₂ and CH₄ uptakes compared to that of CO₂ under the same conditions, suggesting the preferential adsorption of CO₂ over N₂ and CH₄.

The selectivity (S<sub>ads</sub>) performance of the binary mixtures of CO₂/N₂ and CO₂/CH₄ was estimated using the Ideal Adsorbed Solution Theory (IAST), as defined in section 2.3 (eqn (4)). In the 0–1 bar range, the CO₂/N₂ selectivity (Fig. 7e) was calculated considering a typical flue gas composition of 15% CO₂ and 85% N₂, whereas for CO₂/CH₄ selectivity (Fig. 7f), a 50:50 mixture was considered (natural gas sweetening). As shown in Table 5, PCHL-2 demonstrates CO₂/N₂ IAST selectivity factors (at 1 bar) of 36, 35 and 23, while ACP-2-3 exhibits factors of 33, 28, and 16

at 0 °C, 25 °C and 50 °C, respectively. These results indicate that the carbon adsorbent is effective in selectively separating CO₂ from N₂, particularly at the lowest studied temperature (close to 0 °C), where the material demonstrated the highest selectivity. The same IAST selectivity analysis for the CO₂/CH₄ (50:50) mixture shows that at 1 bar pressure and for temperatures ranging from 0 °C to 50 °C, PCHL-2 displays IAST selectivity factors between 14 and 36, whereas ACP-2-3 shows lower factors ranging from 3 to 6. Similar to the CO₂/N₂ mixture, it is evident that the carbon material shows a higher selectivity for CO₂/CH₄ separation at temperatures close to 0 °C.

However, it is noteworthy that the selectivity of the non-activated carbon (PCHL-2) is higher than that of the activated carbon (ACP-2-3), particularly for the separation of a CO₂/CH₄ (50:50) mixture. In fact, materials with smaller average pore sizes are expected to exhibit higher selectivity for CO₂ over CH₄.⁵³ CO₂, which has a higher quadrupole moment than CH₄, interacts more strongly with carbon surfaces within small pores, particularly ultramicropores (<0.7 nm), leading to preferential adsorption.⁵⁴ As shown in Fig. 4b, activation leads to the formation of wider pores in activated carbons compared to the non-activated carbon. This pore enlargement enhances CH₄ adsorption, thereby decreasing CO₂ selectivity. From an industrial perspective, these results suggest the activation step could potentially be omitted from the porous carbon fabrication process. However, other factors must be considered, such as the quantity of adsorbent required, contact time, and additional process parameters that could influence the overall performance and efficiency of an industrial process. Breakthrough curves would be of great interest for process optimization, as they would allow adsorption capacity and selectivity assessment under dynamic flow conditions. From a theoretical standpoint, these results demonstrate that selectivity clearly does not solely depend on the specific surface area but is also likely influenced by other factors such as porous structure and heteroatoms, which undergo alterations during activation and may
<figure><img src="image_15.png" /></figure>

<figure><img src="image_16.png" /><figcaption>Fig. 7 CO₂ and N₂ adsorption isotherms for (a) PCHL-2 and (b) ACP-2-3; CO₂ and CH₄ adsorption isotherms for (c) PCHL-2 and (d) ACP-2-3; IAST selectivity analyses for (e) (15 : 85) CO₂/N₂ mixture and (f) (50 : 50) CO₂/CH₄ mixture, for PCHL-2 (t = 0 h) and ACP-2-3 (t = 3 h).</figcaption></figure>

<table><caption>Table 5 Gas uptakes (CO₂, CH₄, and N₂) at 1 bar and IAST selectivity (CO₂/N₂ and CO₂/CH₄) for PCHL-2 and ACP-2-3</caption><thead><tr><th rowspan="2">Sample</th><th colspan="3">CO₂ uptake [mmol g⁻¹]</th><th colspan="3">N₂ uptake [mmol g⁻¹]</th><th colspan="3">CH₄ uptake [mmol g⁻¹]</th><th colspan="6">IAST selectivity (at 1 bar)</th></tr><tr><th>0 °C</th><th>25 °C</th><th>50 °C</th><th>0 °C</th><th>25 °C</th><th>50 °C</th><th>0 °C</th><th>25 °C</th><th>50 °C</th><th>0 °C</th><th>25 °C</th><th>50 °C</th><th>0 °C</th><th>25 °C</th><th>50 °C</th></tr></thead><tbody><tr><td>PCHL-2</td><td>4.0</td><td>3.2</td><td>1.9</td><td>0.79</td><td>0.43</td><td>0.27</td><td>1.0</td><td>0.8</td><td>0.6</td><td>36.6</td><td>35.4</td><td>23.3</td><td>35.3</td><td>25.0</td><td>13.8</td></tr><tr><td>ACP-2-3</td><td>5.2</td><td>4.0</td><td>2.1</td><td>0.82</td><td>0.49</td><td>0.30</td><td>2.1</td><td>1.0</td><td>1.0</td><td>33.0</td><td>28.0</td><td>16.0</td><td>6.5</td><td>5.7</td><td>3.2</td></tr></tbody></table>

consequently impact selectivity. Further investigation would be required to clearly identify the mechanisms leading to the decrease in selectivity after activation.

Based on all these results, the adsorbent material has demonstrated high CO₂ adsorption capacity and good selectivities for CO₂/N₂ and CO₂/CH₄ separations. Consequently, the
<figure><img src="image_17.png" /><figcaption>Fig. 8 Cyclical CO₂ adsorption behaviour of the ACP-2-3 activated carbon: adsorption at 0 °C and 1 bar, and desorption at 130 °C under vacuum.</figcaption></figure>

porous carbon material developed in the present study is suit-
able for industrial applications in gas separation, such as
natural gas sweetening (CO₂/CH₄ separation) or the removal of
CO₂ from flue gas (CO₂/N₂ separation).

**3.6. Adsorption/desorption cyclability**

Another crucial aspect to investigate for industrial applications
is the stability of the adsorption capacity after multiple
adsorption-desorption cycles. In this study, one cycle con-
sisted of a desorption stage at 130 °C under vacuum to desorb
CO2, followed by an adsorption stage at 0 °C and 1 bar to
measure the CO2 adsorption capacity at equilibrium. The 3Flex
sorption analyser (Micromeritics, Norcross, GA, USA) was used
to evaluate the CO2 adsorption capacity under equilibrium
conditions. This adsorption-desorption cycle was repeated 10
times consecutively on the same activated carbon (ACP-2-3).
The results are presented in Fig. 8 and show that even after
10 cycles, the CO2 adsorption capacity remains stable. This
indicates that ACP-2-3 possesses excellent adsorption-
desorption cyclability, which is of great interest for industrial
applications.

4. Conclusions

This study introduces a straightforward methodology for the fabrication of microporous carbon monoliths from biobased chitosan-PBZ polymers for CO₂ separation. The quantity of chitosan and lysine was found to influence the textural and adsorption properties of the resulting carbon, with medium concentrations providing the most favourable characteristics. Conversely, the char yield remained nearly constant (~49 wt%) for the three concentrations studied.

The thermal activation process significantly enhanced the
adsorption capacity of the porous carbon monolith. A higher
activation progress contributed to greater pore development in

the carbonaceous material, resulting in a notable improvement
in textural characteristics and adsorption capacity. The acti-
vated carbon exhibited a maximum surface area and CO2
uptake of around 1000 m² g⁻¹ and 5.6 mmol g⁻¹, respectively,
with a burn-off of 23%.

Analysis of the available CO₂ adsorption capacity revealed that the activated material achieved the most favourable compromise between increased adsorption capacity and mass loss after a 3 hour activation process (corresponding to a burn-off of 12%). This activated carbon also demonstrated good selectivities for CO₂/N₂ and CO₂/CH₄ separation, with excellent adsorption-desorption cyclability.

A very important result of this work is that activation may
sometimes lead to a decrease in selectivity. This was particularly
evident for the separation of the CO₂/CH₄ (50 : 50) mixture.
From an industrial perspective, this suggests that the activation
step could potentially be omitted from the porous carbon
fabrication process. Further investigation would be required to
clearly identify the mechanisms leading to the decrease in
selectivity after activation.

In summary, the advantages of easy preparation, favourable
surface and adsorption properties, good selectivity and regen-
eration capacity, position the obtained adsorbent carbons (non-
activated and activated) as promising candidates for industrial
CO₂ separation applications.

Data availability

The authors declare that the data supporting the findings of this
study are available within the paper. Should any raw data files
be needed in another format, they are available from the cor-
responding author upon request. Source data are provided in
this paper.

Author contributions

José E. Mosquera: data curation, formal analysis, investigation, methodology, resources, validation, visualization, writing – original draft. Liana Delevingne: data curation, investigation, validation, visualization. Frédéric Delbecq: conceptualization, formal analysis, methodology, writing – review & editing. Elias Daouk: conceptualization, formal analysis, methodology, writing – review & editing. Audrey Drelich: conceptualization, formal analysis, methodology, writing – review & editing. Kha-shayar Saleh: conceptualization, project administration, supervision, writing – review & editing. Rémi Gautier: concep-tualization, funding acquisition, methodology, project admin-istration, writing – review & editing. Mikel Leturia: conceptualization, funding acquisition, methodology, project administration, resources, supervision, writing – review & editing.

Conflicts of interest

There are no conflicts to declare.

<figure><img src="image_18.png" /></figure>
Acknowledgements

The authors gratefully acknowledge the financial support of the Région Hauts-de-France (PISCO Project, dispositif STIMulE, volet Partenarial). They also thank Zaira Hernandez for her invaluable contribution during the preliminary experiments conducted as part of her MSc internship.

References

1 M. W. Jones, G. P. Peters, T. Gasser, R. M. Andrew, C. Schwingshackl, J. Gütschow, R. A. Houghton, P. Friedlingstein, J. Pongratz and C. Le Quéré, *Sci. Data*, **2023**, *10*, 1–23.

2 J. O. Kaplan and M. New, *Clim. Change*, 2006, **79**, 213–241.

3 A. M. Yousef, W. M. El-Maghlany, Y. A. Eldrainy and A. Attia, *Energy*, 2018, **156**, 328–351.

4 G. Singh, K. S. Lakhi, S. Sil, S. V. Bhosale, I. Y. Kim, K. Albahily and A. Vinu, *Carbon*, 2019, **148**, 164–186.

5 X. Ma, Y. Li, M. Cao and C. Hu, *J. Mater. Chem. A*, 2014, **2**, 4819–4826.

6 B. J. Bucior, D. L. Chen, J. Liu and J. K. Johnson, *J. Phys. Chem. C*, 2012, **116**, 25904–25910.

7 M. Sai Bhargava Reddy, D. Ponnamma, K. K. Sadasivuni, B. Kumar and A. M. Abdullah, *RSC Adv.*, 2021, **11**, 12658–12681.

8 I. Tiwari, P. Sharma and L. Nebhani, *Mater. Today Chem.*, 2022, **23**, 100734.

9 A. E. Creamer and B. Gao, *Environ. Sci. Technol.*, 2016, **50**, 7276–7289.

10 X. L. Zhou, H. Zhang, L. M. Shao, F. Lü and P. J. He, *Waste Biomass Valorization*, 2021, **12**, 1699–1724.

11 G. P. Hao, W. C. Li, S. Wang, G. H. Wang, L. Qi and A. H. Lu, *Carbon*, 2011, **49**, 3762–3772.

12 J. Du, W. C. Li, Z. X. Ren, L. P. Guo and A. H. Lu, *J. Energy Chem.*, 2020, **42**, 56–61.

13 T. H. Le and H. Yoon, *Carbon*, 2019, **152**, 796–817.

14 A. C. Lua, F. Y. Lau and J. Guo, *J. Anal. Appl. Pyrolysis*, 2006, **76**, 96–102.

15 C. M. Ghimbeu and V. A. Luchnikov, *Microporous Mesoporous Mater.*, 2018, **263**, 42–52.

16 B. Kiskan, N. N. Ghosh and Y. Yagci, *Polym. Int.*, 2011, **60**, 167–177.

17 N. Liu, L. Shao, C. Wang, F. Sun, Z. Wu, P. Zhan, L. Zhang and H. Wan, *Int. J. Biol. Macromol.*, 2022, **221**, 25–37.

18 M. M. Samy, M. G. Mohamed and S. W. Kuo, *Eur. Polym. J.*, 2020, **138**, 109954.

19 A. A. Alhwaiige, H. Ishida and S. Qutubuddin, *ACS Sustain. Chem. Eng.*, 2016, **4**, 1286–1295.

20 G. P. Hao, W. C. Li, D. Qian, G. H. Wang, W. P. Zhang, T. Zhang, A. Q. Wang, F. Schüth, H. J. Bongard and A. H. Lu, *J. Am. Chem. Soc.*, 2011, **133**, 11378–11388.

21 S. Wang, W. Li, L. Zhang, Z. Jin and A.-H. Lu, *J. Mater. Chem. C*, 2015, **3**, 4406–4412.

22 L. Hong, S. Ju, X. Liu, Q. Zhuang, G. Zhan and X. Yu, *Energy Fuels*, 2019, **33**, 11454–11464.

23 R. Konnola and T. S. Anirudhan, *J. Environ. Chem. Eng.*, 2020, **8**, 103614.

24 T. Takeichi, T. Kawauchi and T. Agag, *Polym. J.*, 2008, **40**, 1121–1131.

25 P. Thirukumaran, A. Shakila Parveen, R. Atchudan and S. C. Kim, *Eur. Polym. J.*, 2018, **109**, 248–256.

26 A. A. Alhwaiige, T. Agag, H. Ishida and S. Qutubuddin, *Biomacromolecules*, 2013, **14**, 1806–1815.

27 Y. Zhu, J. Su, R. Lin, Y. Jiang and P. Li, *Thermochim. Acta*, 2020, **683**, 178465.

28 N. Ramdani, M. Chrigui, J. Wang, T. T. Feng, X. Y. He, W. Bin Liu and X. S. Zheng, *J. Compos. Mater.*, 2015, **49**, 2449–2458.

29 N. Thepphankulngarm, T. Chaisuwan, D. Tanangteerapong and P. Kongkachuichay, *Mater. Chem. Phys.*, 2022, **287**, 126258.

30 Z. E. Jin, J. L. Wang, R. J. Zhao, T. T. Guan, D. D. Zhang and K. X. Li, *New Res. Carbon Mater.*, 2018, **33**, 392–401.

31 A. Hariharan, P. Prabunathan, A. Kumaravel, M. Manoj and M. Alagar, *Polym. Test.*, 2020, **86**, 106443.

32 C. Shaer, L. Oppenheimer, A. Lin and H. Ishida, *Polymers*, 2021, **13**, 3775.

33 L. H. Zhang, W. C. Li, L. Tang, Q. G. Wang, Q. T. Hu, Y. Zhang and A. H. Lu, *J. Mater. Chem. A*, 2018, **6**, 24285–24290.

34 Z. Guo, X. Lu and Z. Xin, *Colloids Surf*, A, 2022, **646**, 128845.

35 Y. Xia, R. Mokaya, G. S. Walker and Y. Zhu, *Adv. Energy Mater.*, 2011, **1**, 678–683.

36 B. Kancı Bozoğlan, O. Duman and S. Tunç, *Colloids Surf*, A, 2021, **610**, 125600.

37 N. Yadav, M. Monisha, R. Niranjan, A. Dubey, S. Patil, R. Priyadarshini and B. Lochab, *Carbohydr. Polym.*, 2021, **254**, 117296.

38 P. I. Morgado, S. P. Miguel, I. J. Correia and A. Aguiar-Ricardo, *Carbohydr. Polym.*, 2017, **159**, 136–145.

39 D. D. Kachhadiya and Z. V. P. Murthy, *J. Environ. Chem. Eng.*, 2023, **11**, 109307.

40 S. Casalini and M. Giacinti Baschetti, *J. Sci. Food Agric.*, 2023, **103**, 1021–1041.

41 T. Witoon and M. Chareonpanich, *Mater. Lett.*, 2012, **81**, 181–184.

42 A. A. Alhwaiige, T. Agag, H. Ishida and S. Qutubuddin, *RSC Adv.*, 2013, **3**, 16011–16020.

43 U. Kamran and S. J. Park, *J. CO2 Util.*, 2020, **40**, 101212.

44 J. E. Mosquera, F. Delbecq, E. Daouk, A. Drelich, K. Saleh, R. Gautier and M. Leturia, *Processes*, 2024, **12**, 1604.

45 M. G. Mohamed, M. M. Samy, T. H. Mansoure, C. J. Li, W. C. Li, J. H. Chen, K. Zhang and S. W. Kuo, *Int. J. Mol. Sci.*, 2022, **23**, 347.

46 F. Liu, K. Huang, Q. Wu and S. Dai, *Adv. Mater.*, 2017, **29**, 1–8.

47 Y. Sun, Z. He, H. Fan and S. Wang, *J. Power Sources*, 2024, **614**, 235027.

<figure><img src="image_19.png" /></figure>
<figure><img src="image_20.png" /></figure>

48 M. Sevilla, J. B. Parra and A. B. Fuertes, *ACS Appl. Mater. Interfaces*, 2013, **5**, 6360–6368.

49 M. J. Teng, Y. S. Wei, T. G. Hu, Y. Zhang, K. Feng, M. H. Zong and H. Wu, *J. Food Eng.*, 2020, **281**, 109993.

50 N. P. Wickramaratne and M. Jaroniec, *ACS Appl. Mater. Interfaces*, 2013, **5**, 1849–1855.

51 K. Yang, J. Peng, H. Xia, L. Zhang, C. Srinivasakannan and S. Guo, *J. Taiwan Inst. Chem. Eng.*, 2010, **41**, 367–372.

52 J. F. Kwiatkowski, *Activated Carbon : Classifications, Properties and Applications*, Nova Science Publishers, New York, 2012.

53 A. Rahimalimamaghani, R. Ramezani, D. A. P. Tanaka and F. Gallucci, *Ind. Eng. Chem. Res.*, 2023, **62**, 19116–19132.

54 N. Yang, S. Liu and X. Yang, *Appl. Surf. Sci.*, 2015, **356**, 1262–1271.